Coupling of synthetic polymers with biological components can greatly increase the variety and complexity of structures originating from polymers. Block copolymers in which one of the building blocks is biological are referred as ‘polymer-bioconjugates’’ or ‘‘macromolecular chimeras’’ introduced by Schlaad et al. . Selection of biological segment does not restrain to one class of molecules- it can be an amino acid or nucleic acid chain (DNA, RNA) as well as an oligo- or polysaccharide. Macromolecular chimeras was the first class of compounds combining convenience of synthetic polymers (e.g. protein repellency, temperature sensitivity) with the features of biological molecules (e.g. targeting-antibodies) .
In order to obtain well defined molecular chimeras, fine control over the synthesis is required.
Synthetic strategies which can be used to obtain polymer bio-conjugates are summed up below.
126.96.36.199 DNA copolymers synthesis
(the following sub-section was adapted with Springer permission from DNA-Polymer Conjugates: From Synthesis, Through Complex Formation and Self-assembly to Applications, Bio-Synthetic Polymer Conjugates by D. Kedracki, I. Safir, N. Gour, N.
Kien Xuan, C. Vebert-Nardin, , 253 (2013) 115-149  and updated with the newest literature)
Modern synthetic chemistry allows currently the versatile synthesis of DNA-polymer conjugates through the large choice over the composition, length and architecture of both oligodeoxynucleotide (ODN) sequences and polymer segments. Conjugation of ODN can be conducted at the 2’-position of the ribose sugar, nucleobases and internucleotidic phosphodiester bonds. But the most common reactions take place at the 5’- or 3’-termini, due to high accessibility of these positions. It has been reported that this strategy has also another advantage, namely conjugation through the 3’-terminus enhances the exonuclease resistance of the nucleotide sequence Conjugation of ODN is considered as quite challenging because even slight changes in the sequence structure may result in its properties change, which is crucial regarding the potential future application of the resulting DNA-polymer conjugates. Therefore, the specific sites for conjugation should be carefully selected. Another issue which has to be considered is that, conjugation sites may have limited access along the ODN fragment. Different stabilities of polymer and nucleotide sequence entities which can occur as the result of their exposure for specific reaction conditions should be also taken under account .
Synthetic strategies of DNA conjugation to polymers mainly rely on coupling terminal groups (grafting strategy), which is presently the most efficient and popular approach. Basically, there are two principal approaches for the binding of an ODN sequence with a polymer, which
can be differentiated into solid-phase synthesis (SPS) and solution coupling. Solution coupling can be used for generation of both water soluble and amphiphilic DNA–polymer conjugates. However, carrying a solution reaction in order to obtain an amphiphilic product usually leads to low yields due to the chemical incompatibility of the two reactants .
These two types of DNA conjugation are based on the same types of reactions. However, despite of the slightly lower coupling efficiency in comparison to the solution coupling, SPS synthesis offers simplified purification and deals better with components solubility. In the last few years new methods of DNA conjugation with polymers have been reported, such as enzymatic reactions, which is not described here and the reader is referred to the following excellent reviews [114-117].
188.8.131.52.1 Solution coupling
Three main routes are used for DNA-polymer conjugation (Figure 1-12):
1) peptide bond formation
Amide bond is formed as a result of reaction between the amino group of one of the reactants (usually DNA) and the carbodiimide (e.g. 1-ethyl-3-(3-dimethylaminopropyl) carbodiimide (EDC)) activated carboxyl group of the second reactant (usually polymer) .
2) disulfide bond formation
This type of conjugation requires both elements modification with sulfhydryl groups, being one of these groups activated .
3) Michael addition
In the case of Michael addition sulfhydryl modification is required as well and this group subsequently reacts with maleimide or acrylic acid. The bond is formed through nucleophilic addition of thiol to an electron deficient carbon .
In the case of all reactions mentioned above the polymer reactant is usually used in slight excess . High yields of DNA-polymer conjugates obtained by solution coupling have been widely reported [120-122]. Needless to say, solution strategies require purification subsequent to coupling.
The most important advantages of solution coupling, which could be accounted for, are that these reactions can be performed in laboratory conditions in a very straightforward way, without expensive automatic DNA synthesizer. Moreover, DNA sequences with various modifications are commercially available.
Figure 1-12. Solution coupling strategies of DNA conjugation with polymers. a) Amide bond formation. b) Formation of disulfide bridges between the thiol groups of both components. c) Michel addition of maleimide to ODNs fragment functionalized with a sulfhydryl terminal group (Figure adapted with permission of Springer)
184.108.40.206.2 Solid-phase synthesis (SPS)
As mentioned above this strategy prevents from performing tedious chemistry and purification steps . It is also noteworthy that, over the course of the SPS reaction, potentially reactive groups along the ODN fragment are protected and thus potential side reactions are excluded. There are two kinds of SPS: programmed, fully automated sequencing in a DNA synthesizer and modified techniques taking advantage of simple tools like syringe filters. The advantages of automated synthesis are precise control over the reaction, large scale and fine reproducibility but the cost of using this approach is quite high. On the other hand, thanks to modified techniques, a product which matches perfectly special needs can be produced  .
Coupling to the 5’-end of ODNs using 2-cyanoethyl-N,Ndiisopropylphosphoramiditite (CEPA) reactive groups (Figure 1-13 A) is the most fundamental method in automated DNA-polymer conjugate synthesis. CEPA modified DNA-polymers react with the detrityleted 5’-end of ODNs bound to a solid support, usually a Controlled Pore Glass (CPG) resin. To couple the polymer segment at the 3’-end of the DNA (Figure 1-13 B), it is necessary to begin with the solid supported polymer or to carry out reverse synthesis, in which the desired compound is attached to the 3’-end of the sequence elongated in the 5’- to 3’-end direction. After cleavage from the resin and deprotection by liquid ammonia, ODN-based copolymers could be achieved .
Figure 1-13. Synthetic scheme of the coupling of DNA with polymers at the (A) 5’- end and (B) 3’-end of the DNA; a ) deblocking of DMT; b)coupling of activated CEPA to the 5’- end;
c) standard synthesis with nucleoside phosphoramidite. Subsequently, in order to obtain the conjugate cleavage from the solid support is conducted prior to the washing out of the 2-cyjoanoethyl groups. (Figure adapted with permission of Springer)
Disadvantages of the synthesis of DNA copolymers without a synthesizer are less convenience and time consumption but it is especially helpful in case of solvents or catalysts incompatibilities. The conditions of post-DNA synthesis indeed change depending on factors such as chemo-stability, catalyst and chemical structures. However, ex-situ approaches allow the preparation of linear and brush-type DNA-polymer conjugates . We briefly present in here the different strategies for ex-situ synthesis on solid support. The mechanisms are the same as in the case of reactions conducted in aqueous solution [116, 123]. A Huisgen reaction occurs between an azide-modified oligonucleotide and an alkyl terminated component to form a 1,2,3-triazole (Figure 1-14 d). This reaction is almost quantitative and can be conducted in aqueous solution. The efficiency of a Huisgen reaction is greatly increased when it is catalyzed by CuI [124, 125]. Sonogashira-Hagihara coupling is a reaction between terminal
alkynes and aryl halide, catalyzed by palladium complexes. The reaction is conducted in the presence of catalytic amounts of CuI and an amine base (Figure 1-14 e) [126, 127].
Figure 1-14. SPS strategies which can be employed for achieving DNA block copolymers (DBCs). a) amide bond formation, b) Michael addition, c) phosphodiester bonding, d) Huisgen reaction, e) Sonogashira-Hagihara reaction. (Figure adapted with permission of Springer)
A recent promising strategy is the “grafting-from” (“blocking-from”) approach which involves DNA chain modification with an initiator from which the polymer chain is grown.
To the main benefits, which can be accounted for, is ease of unreacted species removal as well as purification and higher sterical availability which comes from the nature of the “grafting-from” approach which simply consists in monomer addition reactions . The publications describing ATRP or RAFT polymerization approaches for the synthesis of DNA conjugates appeared already almost 10 years ago [129-131]. These reports depict the growth of the polymer from DNA chains immobilized at the surface modified with a suitable initiator.
Noteworthy, to link the DNA with the appropriate initiator molecule, reactions which are described above are used (the most frequently peptide bond formation, mediated by NHS activation). In the case of the ATRP as well as RAFT polymerization from the DNA chain, an accelerated growth of the polymer chain was observed. This phenomenon was related to the
presence of the highly charged phosphate group and complexation of copper by the nucleotide bases [129, 131]. However, analysis and characterization of the resulting DNA conjugates are problematic due to attachment of the copolymer to the surface. In 2014, Averick et al.
proposed an even less complicated method to generate DNA linked initiators for synthesis of DNA based copolymers. The standard ATRP initiator is indeed converted to phosphoramidite.
The subsequent polymerization occurs through activators generated by electron transfer (AGET) ATRP. This method was shown to provide high control over the molecular weight and narrow molecular weight distribution of the resulting copolymer . It was also demonstrated through hybridization experiments that the nucleic acid sequence preserved its function. Authors evidenced that this strategy allows preparation of hydrophilic (Figure 1-15) as well as amphiphilic DNA based copolymers, which demonstrates the high versatility of this synthetic route. As the initiators were chosen in order to stay intact during the harsh condition of the cleavage from the resin, polymerization can be conducted subsequent or prior to the cleavage. The latter option offers accelerated preparation procedure and simplified purification processes which is especially relevant .
Figure 1-15. Synthesis of DNA based copolymer through AGET ATRP a)deprotection of ODN chain is followed by the addition of ATRP initiator to 5’-OH. Subsequent cleavage results in the deprotected DNA ATRP initiator, b) direct polymerization in solution with the use of two various monomers. (Figure adapted with permission of John Wiley and Sons)
Scope of the thesis
DNA is a remarkable molecule carrying genetic information and involved in a plethora of significant biological processes. Nevertheless, cellular uptake, penetrability and plasma half-life of naked DNA is restricted. In order to overcome these limitations nucleotide sequences were conjugated to hydrophilic synthetic polymers. Coupling to the hydrophobic segments results in formation of nanostructures through self-assembly. This process might affect the properties of DNA involved in the assembly and hence opens new possibilities for carrier designing as well as means to establish the formation mechanism and interaction modes of organized DNA based copolymers. In order to provide such hybrids, synthetic strategies described in the section Synthesis were developed, from which peptide bond formation, maleimide coupling and disulfide bond formation are recognized as the most popular. Due to solubility incompatibility the synthesis of DNA hybrids has been so far evidenced for a finite number of polymer blocks like polystyrene (PS), propylene oxide (PPO), polyfluorene (PFO) and polybutadiene (PB) as the most popular hydrophobic moieties . The structures achieved so far through self-assembly solely are spherical or cylindrical micelles and vesicles.
The microphase separation of the hydrophobic and hydrophilic units was usually the driving force for structure formation .
The presented work deals with the development and characterization of novel DNA based copolymers to enlighten the several fundamental aspects involved in modes of structure formation and interaction. Herein, the others than ordinary ways to drive self-assembly are reported for the first time. Nucleation dependent polymerization as well as emulsification approaches are described. Former path resulted in the fibrillar morphology which is the first example of this particular assembly of DNA based copolymers and the latter produced micrometer size spherical capsules. To the best of our knowledge none of these two approaches was so far utilized in DNA based structure formation. Initially, polymer-DNA
hybrids were prepared according to existing well described chemistry routes; however efforts to establish a novel straightforward strategy to couple DNA with higher efficiency were studied as well. Structures generated from copolymers according to various synthetic routes were investigated varying the hydrophilic weight fraction, and the architecture. Attempts were made to understand the principle of the structure formation of these molecules. In addition for the first time, the interesting bioinspired polymer, namely polyoxazoline was coupled with DNA. Polyoxazolines are regarded as pseudopeptides due to their structural resemblance to natural peptides, which represents their high potential for application in the field of biomedicine. Poly(2-ethyl-2-oxazoline) is an example of polymer of this class which is not toxic, biocompatible and approved by the Federal Drug Administration (FDA).
The thesis is divides into 4 chapters as described below.
3. Self-assembly: Synthesis and Self-assembly of a DNA Molecular Brush
In this chapter, we present a novel synthetic approach to generate of comb/graft DNA based copolymer through one step thiol click chemistry with a high coupling efficiency reaching 60% and high grafting density (67%). We demonstrate that the phenomenon of polymer crystallization can be used at first to simplify the further process of purification. Another important conclusion is that for this specific and high DNA grafting density the resulting copolymer self-assembles intro spherical structures which are stable against hydrogen bonding and as demonstrated by hybridization assays the nucleotide sequences remain functional, which paves the way for the use of this structures for speciation of nucleotide sequences.
4. Hydrogen bonding induced formation of DNA-copolymer fibrils through amyloid-like nucleation polymerization
This chapter describes the synthesis of PBOX-g- DNA copolymers according to conventional chemistry routes. In comparison to the results described in the chapter 3, the so synthesized polymer is of low grafting density, which induces another mode of structure formation. Low grafting density DNA copolymer self-assembles into fibers due to inter-and intramolecular interactions. Investigations of the fibers formation process suggest a nucleation dependent polymerization mechanism, which is very specific for amyloid protein and peptides. This work is of high importance, taking under consideration the association of amyloid fibers with several neurodegenerative diseases such as Alzheimer’s disease.
5. Emulsions and emulsion templated self-assembly
5.1. Polymer-aptamer hybrid emulsion templating yields bio-responsive nanocapsules
It was demonstrated that a suitable DNA copolymer could efficiently stabilize a water-in-oil emulsion. Proven by AFM and reflectometry the functionality of the aptamer (oligonucleotide sequences which bind to a target molecule with very high affinity and specificity) is hindered neither by synthesis nor by the engagement of aptamer in the process of coupling and emulsion stabilization.
5.2. Hybrid Nanocapsules Targeting the Nucleolin Cancer Cells Surface Receptor
Poor solubility of many advanced and effective anticancer drugs is a reason of formulation issues. In order to make delivery of hydrophobic drugs efficient DNA-copolymer stabilized emulsions were further combined with the Layer-by-Layer (LbL) deposition methodology with novel strategy of functionalization with an aptamer. Emulsification would provide simple and highly efficient encapsulation of hydrophobic anticancer drugs.